Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Transcript

June 30, 2010 4:39 World Scientific Review Volume - 9.75in x 6.5in BCS50FFLO Chapter 1 Breaking Translational Invariance by Population Imbalance: The Fulde-Ferrell-Larkin-Ovchinnikov states Gertrud Zwicknagl1 and Jochen Wosnitza2 1 Institut für Mathematische Physik, TU Braunschweig, 38106 Braunschweig, Germany 2 Hochfeld-Magnetlabor Dresden, Forschungszentrum Dresden-Rossendorf, 01314 Dresden, Germany An overview is given of our present understanding of superconductivity with spontaneously broken translation symmetry in polarized Fermi systems. The existence of “crystalline” superconducting phases is considered in a wide range of systems, prominent examples being conduction electrons in metals, ultra-cold atoms in a trap, nuclear matter, and dense quark systems. The underlying physics is delineated and theoretical approaches to the inhomogeneous phases and their properties are discussed. From the experimental side it is argued that superconductivity with imbalance-induced order parameters is realized in layered organic compounds and potentially in heavy-fermion systems. 1.1. Introduction Superfluid phases with unequal numbers of particles forming Cooper pairs have been in the focus of interest for many decades. Of particular interest has been the conjecture by Fulde and Ferrell (FF)1 and Larkin and Ovchinnikov (LO)2 that at low temperatures superfluid states with spontaneously broken translational symmetry should form. These FFLO states have been under theoretical investigation for a variety of systems including metals,3,4 ultra-cold atoms,5 nuclear matter, and dense quark systems.6 In the present review, we shall restrict ourselves to non-relativistic twocomponent Fermi systems, well-known examples being the conduction electrons in metals. In an imbalanced Fermi liquid there will be a majority and a minority component which we shall denote as ↑ and ↓, respectively. The system is characterized by the corresponding densities n↑ ≥ n↓ . For independent particles with no interconversion, the densities of the majority and minority degrees of freedom, n↑ and n↓ , can alternatively be specified by chemical potentials µ↑ and µ↓ . The latter are expressed by the average value and the difference µ↑ = µ + δµ ; µ↓ = µ − δµ 1 . (1.1) June 30, 2010 4:39 2 World Scientific Review Volume - 9.75in x 6.5in Gertrud Zwicknagl and Jochen Wosnitza In spin-1/2-fermion systems, such as the conduction electrons in metals, the difference in the chemical potentials, δµ, is tuned by an external magnetic field. In trapped atomic systems, on the other hand, imbalance can be generated by preparing mixtures with different numbers of partners and the natural variable is the polarization, i.e., the difference in the corresponding particle numbers. Due to the formation of Cooper pairs the susceptibility of the superconductor is reduced as compared to the normal state. For high differences in the chemical potentials the polarized normal state has a lower energy than the superconducting phase. Qualitatively, the transition from the paired superconducting to the polarized normal phase will occur when the polarization energy equals the condensation energy of the Cooper pairs. This condition defines the limiting chemical-potential mismatch, δµc (T ), beyond which homogeneous superconductivity will not exist. The low-temperature limit δµc (0) for a conventional superconductor was first given by Chandrasekhar7 and Clogston8 ∆0 δµc (0) = √ , 2 where ∆0 is the energy gap of the uniformly balanced reference system. The δµ-T phase diagram for homogeneous superconductors was studied in detail by Sarma.9,10 In addition to the normal phase and the BCS solution, he considered a compromise state which embodies “phase separation in momentum space”. The breached-pair (BP) states11 are characterized by the coexistence of paired superfluid and normal polarized components which reside in different regions of momentum space. Unfortunately, these gapless states turn out to be unstable in the “classical” situation of a superconductor in an external magnetic field acting on the spins of the electrons. The interest in BP states, however, has been recently rekindled since they could be realized in dense quark systems or ultra-cold atoms. FFLO predicted a spatially inhomogeneous partially gapped compromise state with both paired superfluid and normal polarized regions to be the stable ground state in a (narrow) range above the Chandrasekhar–Clogston limit. The idea of forming a textured state with paired and normal regions closely parallels the concept of the vortex phase which appears in type-II superconductors below the upper critical field. This phase gains its stability from the fact that it allows magnetic flux to penetrate into the superconductor. Like the FFLO state, it was predicted theoretically by Abrikosov.12 Shortly afterwards, it was confirmed by numerous experiments employing a variety of techniques. Although the existence of inhomogeneous compromise states in imbalanced superfluids seems plausible and despite intensive search, these phases have not yet been identified unambiguously. There are, however, indications that they are realized in some highly anisotropic materials, as will be discussed below. There are several reasons for the difficulties in the experimental observation. First, the FFLO state requires very stringent conditions which strongly restrict the appropriate classes of superconducting materials. Soon after the FFLO phases BCS50FFLO June 30, 2010 4:39 World Scientific Review Volume - 9.75in x 6.5in Breaking Translational Invariance by Population Imbalance BCS50FFLO 3 were conjectured it became clear that impurities act as pair breakers suppressing the corresponding transition temperatures.13 A necessary criterion for the realization of an FFLO state is a long mean-free path exceeding the superconducting coherence length. An additional technical difficulty encountered in metals is related to the fact that electrons are charged particles. An external magnetic field required to create the imbalance in the conduction electron system will inevitably act on their orbits and suppress superconductivity. To observe imbalance-induced high-field phases the orbital pair breaking must be strongly reduced as pointed out by Maki.13 The early search for the FFLO phases concentrated on thin superconducting films in parallel magnetic fields.14 Although polarization effects were clearly seen it was not possible to stabilize the FFLO state. Promising candidates are recently discovered heavy-fermion compounds and the layered organic superconductors. Second, there are no simple criteria which could help to identify the phases. The order parameter as such is a quantum mechanical object and hence cannot be observed directly. The generally accepted procedure in this situation is to calculate observable properties which depend on the order parameter and hence reflect its structure. It turns out, however, that the properties of FFLO states are non-universal depending sensitively on the normal state, i.e., the dispersion of the quasiparticles and their interactions. The latter strongly affect the transition line separating the normal and the superfluid phases as well as the order of the phase transitions. In addition, the anisotropy of the order parameter in the homogeneously balanced phase which is related to the presence or absence of low-energy excitations plays an important role. Considering these complications, the present article does not attempt at providing a final answers as to the existence and potential realization of imbalancedinduced spontaneous breaking of translational symmetry. The central goal is to summarize basic concepts and discuss the present state-of-the-art emphasizing what were solved and what should be solved. The article is organized as follows: In Section 1.2, we briefly review the groundstate properties of a superconductor with population imbalance. The properties of inhomogeneous phases are summarized in Section 1.3. In Section 1.4, we comment on the experimental situation with an emphasis on condensed-matter systems. The article closes with a summary and an outlook in Section 1.5. 1.2. Theoretical background 1.2.1. Order parameter The highly correlated superfluid phases in a multi-component Fermi liquid are characterized by long-range order in the two-particle density matrix which allows us to define order parameters ΨAB (x, x0 ) = hψA (x)ψB (x0 )i . (1.2) June 30, 2010 4:39 4 World Scientific Review Volume - 9.75in x 6.5in Gertrud Zwicknagl and Jochen Wosnitza The indices A and B denote (pseudo) spins in the case of electron systems or 3 He, for ultra-cold atoms they refer to hyperfine states, whereas they include color, spin, and flavor indices in quark condensates. In the two-component systems to be considered here, the pair amplitudes Eq. (1.2) depend upon the fermion spins and positions which are conveniently ex1 0 pressed in terms of the ¡ center-of-mass ¢ and relative coordinates R = 2 (x + x ) 1 1 0 and r = x − x , Ψσσ0 R + 2 r, R − 2 r . We focus on the BCS regime where the characteristic time and length scales in superconducting phenomena, set by the inF verse gap function ∆−1 and the coherence length ξ0 = ~v π∆ , respectively, are very large on the atomic scale determined by the inverse Fermi energy EF and Fermi wavelength λF . This separation of length and time scales allows us to classify the order parameter of inhomogeneous systems in close analogy to their homogeneous counterparts. In homogeneous superconductors the order parameter is a function of the relative variable only. It varies on the scale of the Fermi wavelength which follows from the short-ranged character of the attractive quasiparticle interaction. Performing a Fourier transformation with respect to r with Ψσσ0 (r) → Ψσσ0 (k) and restricting the wave vector to the Fermi surface kF yields a pairing amplitude Ψσσ0 (kF ) which depends upon the direction kF on the Fermi surface. The fundamental property of Ψσσ0 is its behaviour as a two-fermion wave function in many respects. This expresses the fact that a superconducting order parameter is not the thermal expectation value of a physical observable, but rather a complex (pseudo) wave function describing quantum phase correlations on the macroscopic scale of the superconducting coherence length. Its phase is a direct signature of the broken gauge invariance in the superconducting condensate. The Pauli principle requires Ψσσ0 to be antisymmetric under the interchange of particles Ψσσ0 (kF ) = −Ψσ0 σ (−kF ). In addition, it transforms like a two-fermion wave function under rotations in position and spin space and under gauge transformations. The transformation properties yield a general classification scheme for the superconducting order parameter which is represented by a 2 × 2 matrix in (pseudo) spin space. It can be decomposed into an antisymmetric “singlet” (s) and a symmetric “triplet” (t) contribution according to Ψ(kF ) = Ψs (kF )+Ψt (kF ) with P3 Ψs (kF ) = φ(kF )iσ2 and Ψt (kF ) = µ=1 dµ (kF )σµ iσ2 , where σµ denote the Pauli matrices. Antisymmetry, Ψ(kF ) = − ΨT (−kF ), requires φ(kF ) = φ(−kF ) and dµ (kF ) = −dµ (−kF ) for the complex orbital functions φ(kF ) and dµ (kF ) with µ = 1, 2, 3. The general classification scheme for superconducting order parameters proceeds from the behavior under the transformations of the symmetry group G of the Hamiltonian. It consists of the crystal point group G or the SO(3) in the case of an isotropic liquid, the spin-rotation group SU(2), the time-reversal symmetry group K, and the gauge group U(1). A comprehensive description is given e.g. in Ref. 15 and references therein. BCS50FFLO June 30, 2010 4:39 World Scientific Review Volume - 9.75in x 6.5in Breaking Translational Invariance by Population Imbalance BCS50FFLO 5 Population imbalance affects only opposite “spin” pairs, i.e., pairs formed by different species which occur in the even-parity (spin-singlet) superconductors as well as the dz -component of a triplet state. In the following discussion, we shall focus on even-parity (spin-singlet) superconductors belonging to a one-dimensional representation Γ of the symmetry group. These states are characterized by a complex scalar function, g (kF ), which can have zeros, symmetry-imposed or accidental, on the Fermi surface. If Γ is the unity representation, the superconductor is called “conventional”, otherwise we call it “unconventional”. The classification scheme described above refers to the symmetry properties of the pair amplitudes with respect to the relative variable which reflects the shortranged quasiparticle interaction varying on the atomic scale. Considering the separation of length scales we adopt the same scheme to classify the variation with the relative variable of inhomogeneous order parameters speaking of s- and d-wave, conventional and unconventional FFLO states. A textured order parameter which varies periodically with the center-of-mass variable R on the scale of the coherence length may break both translational and rotational symmetry. The general classification scheme for periodic order parameter has not yet been worked out. An interesting phenomenon is the potential spontaneous breaking of relative symmetries in FFLO states. The orientation of the “crystalline” order parameter is determined by anisotropies of the normal state properties but also by anisotropies in the order parameter of the homogeneous reference system. 1.2.2. Population imbalance and breaking of translational symmetry To start with, we consider a two-component Fermi liquid at T = 0 where the two species are denoted by ↑ and ↓, respectively. The elementary excitations in the normal state are weakly interacting quasiparticles with dispersion ²(k) where the energies are conveniently measured relative to the average chemical potential µ. The quasiparticles feel a short-ranged attraction V which causes the instability of the normal state. Adopting mean-field approximation and introducing the abbreviation D E X 0 ∆ (k; q) = V (k, −k; k0 , −k0 ) c−k0 + q2 ↓ ck0 + q2 ↑ (1.3) k0 for the effective pair field leads to the separable model Hamiltonian16 X H= H (k) + const , (1.4) k where ³ ³ ´ ³ ³ ´ q´ q´ H (k) = ² k + − δµ c†k+ q ↑ ck+ q2 ↑ + ² −k + + δµ c†−k+ q ↓ c−k+ q2 ↓ 2 2 2 2 +∆∗ (k; q) c−k+ q2 ↓ ck+ q2 ↑ + ∆ (k; q) c†k+ q ↑ c†−k+ q ↓ . (1.5) 2 c†kσ 2 The operators (ckσ ) create (annihilate) a quasiparticle in state kσ, δµ denotes the chemical potential mismatch. In Eq. (1.4), the constant corrects for double June 30, 2010 4:39 6 World Scientific Review Volume - 9.75in x 6.5in Gertrud Zwicknagl and Jochen Wosnitza counting of interactions. An ultraviolet cut-off is introduced as indicated by the prime in the sum. As written, Eq. (1.5) is the usual BCS Hamiltonian for an order parameter with finite center-of-mass momentum q varying in real space ∼ eiq·R .17,18 We assume that the corresponding length scale is set by the coherence length ξ0 which implies q ∼ 1/ξ0 ¿ kF . In that respect, the modulated order parameters considered here differ from those of antiferromagnetic superconductor19,20 where the staggered field induces contributions hc−k0 + q2 ↓ ck0 + q2 ↑ i with q ∼ kF .21 The thermodynamic properties of the model Eq. (1.4) can be deduced from the free energy. For a given chemical-potential mismatch the latter is calculated by treating the center-of-mass momentum q and the pair potential ∆ (k; q) as variational parameters. The values of the latter are subsequently determined so as to minimize the free energy. Proceeding along these lines yields directly the (meta-) stable states. The traditional approach based on solving the self-consistency equation for the order parameter yields the stationary points of the free energy which include (meta-) stable as well as unstable phases. Following this line of thought we begin by calculating the eigenvalues and eigenstates of the model Hamiltonian for a given chemical-potential mismatch δµ, centerof-mass momentum q, and pair potential ∆ (k; q). Since all pair Hamiltonians H(k) commute the eigenfunctions of the BCS Hamiltonian Eq. (1.4) will be products of the eigenstates of the H(k). The operators H(k) are easily diagonalised in the basis c†k+ q ↑ |0i, c†−k+ q ↓ |0i, c†k+ q ↑ c†−k+ q ↓ |0i, 2 2 2 2 and |0i where the single-particle states |k; ↑i and |k; ↓i are eigenstates with energies ¢ ¡ ¢ ¡ Ek↑ = ² k + q2 − δµ and Ek↓ = ² −k + q2 + δµ, respectively. The characteristic feature of the superconducting state are the pair states |k; −i and |k; +i with q 2 2 energies E∓ (k) = ² (k) ∓ (² (k)) + |∆ (q; k)| , which are obtained as coherent superpositions of the two-particle states and the empty state in close analogy to bonding and anti-bonding states in molecular physics. We explicitly used the fact that the anticipated center of mass momentum of ¢the Cooper pairs ¡ ¡ ¡ ¢¢ is small on the scale of the Fermi momentum setting 21 ² k + q2 + ² −k + q2 ' ² (k). Transitions between the different branches labeled by ν = ±, ↑, ↓ are described in terms of ladder operators, the Bogoliubov operators. Fig. 1.1 displays the eigenvalues for the unperturbed balanced superconductor (a) and one with imbalance and finite center of mass momentum (b) and (c). In the unperturbed superconductor, the bound pair states |k; −i are energetically more favorable than the single particle states. Both the chemical potential mismatch δµ and finite center-of-mass momentum q, shift the single-particle state relative to the bound pair states which remain unaffected. For a fixed direction on the Fermi surface, δµ and ~2 vF (kF ) · q can be combined to mutually compensate the shifts. The appropriate q-vector depends, of course, on the Fermi velocity vF (kF which varies on the Fermi surface. As a consequence, it is impossible to fully compensate a mismatch δµ for all fermions at the Fermi surface in two-dimensional (2D) and 3D superconductors by choosing a single wave vector q. Depending on the relative size BCS50FFLO June 30, 2010 4:39 World Scientific Review Volume - 9.75in x 6.5in Breaking Translational Invariance by Population Imbalance BCS50FFLO 7 ¯ ¯ of ¯δµ − ~2 vF (kF ) · q¯ and ∆ (k; q) we may have partial compensation (see Fig. 1.1(b)) and even overcompensation (see Fig. 1.1(c)) where minority states ↓ are energetically most favorable in parts of momentum space. In a 1D superconductor, on the other hand, the mismatch δµ can be fully compensated resulting in the absence of a limiting δµ value. Fig. 1.1. Eigenvalues Eν with ν = −, ↑, ↓, + of the pair Hamiltonian Eq. (1.5) for ∆ > 0 vs kinetic energy ²(k) of the normal-state quasiparticles. In a homogeneous superconductor without imbalance (δµ = 0, q = 0, i.e., Q = 0) (left panel) the ground state is formed as a product of bound-pair states, i.e., ν (k) = − or all momenta k. Population imbalance δµ > 0 in a homogeneous superconductor as well as finite center-of-mass momenta q 6= 0, i. e., Q 6= 0, (middle and right panel) may reduce the energies of the single particle states E↑(↓) below those of the bound-pair states. The Zeeman splitting may be partially compensated by finite center-of-mass momentum. Forming a many-particle state with single-particle states in the vicinity of the Fermi energy ξ = 0 reduces the phase space for pairing. At the intersection of the branches, the character of the compromise state changes abruptly. This leads to singularities in the ground-state energy as function of ∆, δµ, and q. Having diagonalized the mean-field Hamiltonian for arbitrary ∆, δµ, and q we now turn to a discussion of the ground state of the system which – like any eigenstate of the model Hamiltonian Eq. (1.4) – is given as a product |Ψ {ν (k)}i = Q k |k; ν(k)i. The index function ν (k) = ∓, ↑, ↓ specifies the state to be selected for a given k-vector. At this point we would like to emphasize that the product must run over all k states in order to obtain an eigenfunction of the model Hamiltonian. This feature reflects the highly correlated nature of the states. Any eigenstate is characterized by the momentum-space function ν (k) which can be viewed as an analogue of the momentum-distribution function. The corresponding energy, given by X Eν(k) (k) , (1.6) E ({ν (k)}) = k is minimal when the state ν0 (k) with the lowest value for every k is selected. Comparing the energies of the bound pair states E− (k) to those of the single-particle states E↑ (k) and E↑ (k) in Fig. 1.1 shows that the BCS wave function built as a Q product of bound pair states |Ψ0BCS i = k |k; −i gives the lowest energy for weak imbalance (δµ < ∆) and long-wavelength modulation ( ~2 vF q < ∆). June 30, 2010 4:39 World Scientific Review Volume - 9.75in x 6.5in 8 BCS50FFLO Gertrud Zwicknagl and Jochen Wosnitza The central focus of the present article are compromise states built from a combination of bound pair states and single-particle states. These states include the gapless homogeneous BP phase where the normal majority component is found in the immediate vicinity of the Fermi surface. Allowing for finite center-of-mass momentum q, we arrive at partially gapped states where quasiparticle excitations of both the majority and the minority components may be present at kF . The gapless regions do not contribute to pairing, they are “blocked”. In general, blocking reduces the energy gain due to pair formation and, consequently, destabilizes the superfluid state. Treating ∆ and q as independent variables, the energy gain due to pair formation for given δµ is easily evaluated from ∆ES (∆, δµ, q) = X X 0 minν Eν (k) − (² (k) + σδµ) Θ (− (² (k) + σδµ)) + const , k (1.7) k,σ with the Heaviside function Θ(x) = 0 for x < 0 and Θ(x) = 1 otherwise. The first two terms are the quasiparticle contribution while the constant corrects for double counting of interaction energies in the quasiparticle contribution. Before we turn to the solution we simplify the notation and introduce dimensionless variables. We explicitly account for the fact that the relevant degrees of freedom are restricted to the immediate vicinity of the Fermi surface. As a result, the summation over the quasiparticle states separate into products of integrals over the Fermi surface parameterized by kF and energy integrations over ξ X k Z . . . = N (0) ¿Z Z w (kF ) dkF dξ . . . = N (0) À dξ . . . . (1.8) FS We R introduced h. . .iF S as a short-hand notation for the Fermi-surface integral w (kF ) dkF . . . with the normalized weight function hw (kF )iF S = 1 given by the 1 Fermi velocity w (kF ) ∝ |vF (k . This allows us to fully account for anisotropies F )| in the Fermi wave vector and in the effective mass. The anisotropic gap E function is D 2 given by ∆ (q; kF ) = ∆q g (kF ) with the normalized function |g (kF )| = 1. All energies are measured in units of the order-parameter amplitude ∆0 which minimizes the energy difference Eq. (1.7) of the homogeneous reference system q = 0 F )·q and measure the centerwithout imbalance δµ = 0. We define Q (kF ) = ~vF (k 2 of-mass momentum in units of the inverse coherence length. Finally, the coupling constant and the ultra-violet cut-off are eliminated in favor of the energy gap ∆0 June 30, 2010 4:39 World Scientific Review Volume - 9.75in x 6.5in Breaking Translational Invariance by Population Imbalance BCS50FFLO 9 and we arrive at ∆ES (∆q , δµ, q) /N (0) = D E 1 2 2 − |∆q | + (δµ + Q (kF )) 2* FS + r ³ ´ 2 2 2 2 − Re (δµ + Q (kF )) (δµ + Q (kF )) − |∆q | |g (kF )| q * + |∆q | 2 2 |g (kF )| Re log FS q 2 2 2+ (δµ + Q (kF )) + (δµ + Q (kF )) − |∆q | |g (kF )| 2 ∆0 |g (kF )| FS (1.9) The expression has singularities which correspond to the bounds of the brokenpair regions. This fact already indicates that an expansion of the ground-state energy in terms of the order-parameter amplitude ∆ is likely to fail. The radius of convergence of such an expansion will depend upon the dimensionality of the system under consideration. The consequences were discussed in detail by Combescot and Mora.22 Fig. 1.2. Contour plot of variation with δµ and ∆ of the energy gain ∆ES (∆q=0 , δµ, q = 0)/(N (0)∆20 ) (see Eq. (1.7)) for the homogeneous s-wave (left panel) and dx2 −y2 - (right panel) superconductor. Solutions of the self-consistency equation correspond to stationary points of ∆ES with respect to variations of ∆q=0 . The order-parameter amplitude ∆q=0 and the chemicalpotential mismatch δµ are measured in units of the order-parameter amplitude ∆0 in the BCS ground state of the corresponding unperturbed reference system. The latter corresponds to the minimum of ∆ES along the δµ = 0-line. For the homogeneous s-wave state, ∆ES has a (local) minimum at ∆/∆0 = 1 as long as δµ/∆0 < 1. The BCS state (solid line) therefore persists as a (meta-) stable state up to the superheating “field” δµ/∆0 = 1. For small values of the mismatch δµ/∆0 < 0.5, the BCS state is the only minimum of ∆ES . At the supercooling “field” δµ/∆0 = 0.5, the normal state ∆/∆0 = 0 becomes a (local) minimum. The homogeneous systems exhibit a rather broad two-phase regime for 0.5 ≤ δµ/∆0 ≤ 1. In this δµ-range, ∆ES has a local maximum which corresponds to Sarma’s unstable solution of the self-consistency equation (dashed line). The qualitative behavior of ∆ES for a homogeneous dx2 −y2 order parameter closely parallels that of the homogeneous isotropic s-wave superconductor. The quantitative differences, however, are due to the presence of low-energy quasiparticle excitations. June 30, 2010 4:39 10 World Scientific Review Volume - 9.75in x 6.5in BCS50FFLO Gertrud Zwicknagl and Jochen Wosnitza The evolution of the ground-state energy of a homogeneous superconductor with imbalance is displayed in Fig. 1.2 for a homogeneous isotropic s-wave superconductor and its dx2 −y2 -counterpart. The characteristic features can be summarized as follows: For large values of the chemical-potential mismatch δµ > ∆0 , the energy increases monotonically with ∆ and the normal state ∆ = 0 is the only stable phase. As δµ is lowered below δµ = ∆0 , the BCS gound state ∆ = ∆0 appears as a metastable state and we enter the two-phase regime. The latter extends down to the supercooling field δµ = ∆20 below which the system must be superconducting. In the two-phase regime, the local minima, i.e., the normal state ∆ = 0 and the usual BCS q state ∆ = ∆0 , are separated by a well which is centered at the line ∆ = ∆0 δµ 2∆ − 1 which was found by Sarma.9 At the Chandrasekhar–Clogston 0 ∆0 limit, δµ = √ , the normal phase and the BCS state become degenerate and a 2 first-order transition between the normal and the superconducting state occurs. It is important to note that there is no stable BP state, superconducting (meta-) stable states occur only for ∆ = ∆0 ≥ δµ. The main features are also present in the case of a dx2 −y2 order parameter which is likely to occur in many superconductors with strongly correlated electrons. The presence of low-energy excitations, however, reduces the energy-gap opening at the superheating field. We next turn to the case of finite-q pairing. As pointed out before, the possible compensation of the chemical-potential mismatch depends on the dimensionality of the system. This is clearly evident from Fig. 1.3 which shows the regions in δµ-q-∆ space where the energy of the superconducting state is lower than that of the normal phase, ∆ES (∆q , δµ, q) ≤ 0, for isotropic 3D and 2D as well as for 1D superconductors with s-wave order parameter. The limiting value ∆µc (T ) is given by the maximum which only slightly exceeds the Chandrasekhar–Clogston limit in 3D. In 2D, the limiting value is enhanced and coincides with the beginning of the two-phase regime. The singularities for small ∆ give rise to highly anomalous properties to be discussed in the subsequent section. The absence of a limiting mismatch in 1D is obvious. At finite temperatures T > 0, the free-energy gain due to pairing is given by · D E T 2 2 + |∆q | ln ∆F (∆q , δµ, q; T ) = −N (0) − (δµ − Q (kF )) Tc0 FS ¿q À ∞ µ X 2 2 2Re +2πkB T (ω` + i (δµ − Q (kF ))) + |∆q | g 2 (kF ) `=0 2 −2ω` − |∆q | ω` FS !# , where ω` = πkB T (2` + 1) are the fermionic Matsubara frequencies and Tc0 denotes the superconducting transition temperature of the unperturbed reference system. Of particular interest is the second-order transition from the normal phase to a superconducting state ∆q eiq·r which occurs at a critical mismatch δµ(T ) given (1.10) June 30, 2010 4:39 World Scientific Review Volume - 9.75in x 6.5in Breaking Translational Invariance by Population Imbalance BCS50FFLO 11 Fig. 1.3. Variation with chemical-potential mismatch δµ/∆0 , order-parameter amplitude ∆q /∆0 , and length of modulation vector Q = ~2 v∆F q of the energy difference ∆ES from Eq. (1.9) for (a) an 0 isotropic three-dimensional (3D), (b) an isotropic two-dimensional (2D), and (c) one-dimensional Fermi surface. All energies are measured in units of the order-parameter amplitude ∆0 characterizing the BCS ground state of the homogeneous (q = 0) unperturbed (δµ = 0) reference system. In the filled regions, the superconducting solution is energetically more favorable than the normal state (∆ES < 0). The boundary surface corresponds to combinations of δµ/∆0 , ∆q /∆0 , and Q = ~2 v∆F q for which the energy of the superconducting solution equals that of the normal state, 0 √ i. e., ∆ES = 0. The plane δµ/∆0 = 1/ 2 corresponds to the Chandrasekhar-Clogston limit for the first-order transition between the homogeneous superconducting and normal states. For modulated states Q 6= 0, pair formation can lead to energy gain for chemical-potential mismatch δµ/∆0 exceeding the Chandrasekhar-Clogston limit. by the linearized selfconsistency equation (linearized stationarity condition) for ∆F (∆q , δµ, q; T ). The latter is given by the implicit equation µ ¶ ¿ µ ¶À T 1 1 1 2 ln =ψ − minQ g (kF ) Re ψ +i (δµ (T ) + Q (kF )) , Tc0 2 2 2πkB T FS (1.11) where ψ (z) is Euler’s digamma function. The optimal modulation vector depends on the anisotropies of the normal-state quasiparticle dispersion and the superconducting order parameter as given by vF (kF ) and g (kF ). The variation with T has been analysed in great detail by Saint-James and Sarma10 for the s-wave case. The formal ¡ key¢ to the phase diagram is the variation with x of the curvature −Re ψ 00 12 + ix which is negative for small values of the argument and changes sign at x = 0.304. This implies that close to the transition temperature Tc0 , i.e., for small values of δµ the homogeneous state q = 0 is formed. In this temperature range the critical mismatch follows a universal curve independent of the details of the system under consideration. With decreasing temperature a tricritical point appears at T = 0.55Tc0 , below which the transition from the normal state into a modulated state with q 6= 0 occurs. The critical value for the mismatch assuming q = 0 becomes the supercooling field below which the homogeneous superconductor is the thermodynamically stable phase. The influence of dimensionality on the δµ-T phase diagram is clearly evident 4:39 World Scientific Review Volume - 9.75in x 6.5in 12 BCS50FFLO Gertrud Zwicknagl and Jochen Wosnitza from Fig. 1.4 (left panel) which displays the variation with temperature of the critical mismatch for s-wave superconductors with spherical and cylindrical Fermi surfaces as well as the two-phase regime for homogeneous superconductivity bounded by the superheating and the supercooling fields as well as the corresponding line of first-order transitions. In an anisotropic superconductor nodes of the gap function select the optimal orientation of the modulation vector q. The latter may change discontinuously with temperature leading to kinks in the critical-field curve. This effect was predicted for superconductors with a dx2 −y2 order parameter and a cylindrical Fermi surface by Maki and Won23 as shown in Fig. 1.4 (right panel). 1.2 1.0 normal state 2−phase 0.5 0.4 homogeneous superconductor 0.0 0.0 0.5 T/Tc normal state 0.8 δµ/∆ 0 δµ/∆ 0 June 30, 2010 homogeneous superconductor 1.0 0.0 0.0 0.5 T/Tc 1.0 Fig. 1.4. Comparison of δµ-T phase diagrams. Left panel: s-wave superconductor. For temperatures above the tricritical point (black dot) the normal state becomes unstable relative to a homogeneous superconducting state (for sufficiently low δµ). Below the tricritical point, the homogeneous superconducting phase can coexist with the normal state in a δµ regime bound by the supercooling field (dotted line) and the superheating field. In a 3D system with spherical Fermi surface a second-order transition from the normal state to an FFLO state (solid line) is found for δµ slightly above the critical value for the first-order transition between the homogeneous phases (dashed line). For a 2D system with cylindrical Fermi surface the second-order transition (dash-dotted line) coincides with the superheating field of the homogeneous phases. Right panel: d-wave superconductor. Second-order transition from the normal to the dx2 −y2 FFLO state in a 2D superconductor with cylindrical Fermi surface for modulation vector parallel to the nodal direction (dashed line) and anti-nodal direction (solid line). The supercooling field (dotted line) is included for comparison. The second-order transition lines give good qualitative insight into the overall behavior of superconductors with population imbalance. The explicit evaluation of the full phase diagram including potential first-order transitions requires the calculation of the free energy for general inhomogeneous order parameters. 1.3. Properties of the inhomogeneous states At sufficiently low temperatures, the polarized normal state of an unbalanced Fermi liquid should become unstable against an inhomogeneous superconducting state. June 30, 2010 4:39 World Scientific Review Volume - 9.75in x 6.5in Breaking Translational Invariance by Population Imbalance BCS50FFLO 13 The modulation vector minimizing the free energy, however, is not unique. Usually, there are several equivalent modulation vectors qm , with m = 1, . . . , M , in agreement with the point-group symmetry of the underlying crystal. In the vicinity of the second-order transition, the corresponding plane-wave order parameters ∼ eiqm ·R are equivalent. In idealized isotropic systems, all plane-wave states ∼ eiq·R with the same wavelength are degenerate at the transition. In the fully developed superfluid phase below the transition this degeneracy is lifted by non-linear terms as shown by Larkin and Ovchinnikov.2 Forming linear combinations of the equivalent plane-wave states results in an order parameter whose amplitude is periodically modulated which results in “crystalline” superconductivity. Determining the optimal spatial structure of the periodic order parameter and predicting the properties of the corresponding superconducting phase is a problem which has been solved only partially. An adequate microscopic analysis of the nonuniform FFLO phases requires simultaneous selfconsistent calculations of the following properties which are intimately intertwined: (i) the inhomogeneous order parameter structure, (ii) the local excitation spectrum, and (iii) the quasiparticle selfenergy accounting for the renormalizations and Fermi-liquid interactions. The technical difficulties are associated with the fact that often there is a great number of different yet energetically almost degenerate states. 1.3.1. Mean-field results: Quasiclassical theory A suitable framework for a numerical study of the complete phase diagram of inhomogeneous superconductors is the quasiclassical theory of superconductivity developed by Eilenberger, Larkin and Ovchinnikov, and Eliashberg (ELOE).24–26 The quasiclassical theory of superconductivity is valid on the coarse-grained length and time scales of the superconducting phenomena set by the coherence length ξ0 = ~vF /π∆0 and the inverse gap frequency ∆−1 . At the outset, properties determined by the Fermi wavelength kF−1 and the Fermi energy ²F are explicitly eliminated from the theory. We would like to emphasize that, since the traditional BCS theory is restricted in accuracy to terms of order Tc /²F an advantage of the quasiclassical method is that it acknowledges this fact and eliminates as many intermediate steps as possible. For the special case of a superconductor close to the transition point a quasiclassical description was derived by deGennes.27 The quasiclassical theory of ELOE is based on formal many-body perturbation theory, expressed in terms of the thermodynamic (imaginary time) Green’s function G(x, x0 ; iωn ). Here G is a 4 × 4 Nambu–Gorkov matrix Green’s function28,29 which contains the “anomalous” Green’s functions in the off-diagonal quadrants. In what follows, only the static limit will be important, and, consequently, only one frequency, the energy variable, appears as an argument. In the first step, center-of-mass and relative variables are introduced and a Fourier transformation ¢ ¡ with respect to the latter is performed G R + 21 r, R − 12 r; iωn −→ G (k, R; iωn ) The central quantity of the theory is the “quasiclassical” or “ξ-integrated” Green’s June 30, 2010 4:39 14 World Scientific Review Volume - 9.75in x 6.5in Gertrud Zwicknagl and Jochen Wosnitza function g(kF , R; iωn ) which is derived from the full propagator G (k, R; iωn ) by averaging over the kinetic energy of the quasiparticles. The equations determining g(kF , R; iωn ) take the form of transport-like equations which are supplemented by a normalization condition. For a comprehensive review see Ref. 30. The quasiclassical method was successfully used to study the evolution of FFLO states characterized by one-dimensional stripe patterns for the order parameter. For quasi-2D s-wave superconductors, Burkhardt and Rainer31 examined selfconsistently the FFLO state including Fermi-liquid interactions. An important result is that the transition from the inhomogeneous FFLO state to the uniform superconducting phase should be of second order. The authors showed that both the critical value of the chemical-potential difference as well as the order of the normal-tosuperconducting phase transitions sensitively depend upon the isotropic exchange interaction among the quasiparticles. Variation with temperature of the order of the normal-to-superconducting transition was also found for isotropic 3D s-wave superconductors by Matsuo et al.32 and confirmed by Combescot and Mora.22 The full phase diagram for a dx2 −y2 order parameter in an isotropic quasi-2D superconductor was studied by Vorontsov et al.33 In unconventional superconductors, the orientation of the stripe pattern relative to the nodal direction of the gap can vary discontinuously with temperature.23,34–36 The change in the modulation vector q is found below T ∗ ' 0.06Tc . Concerning the identification of FFLO phases, Vorontsov et al.33 suggest to measure the Andreev resonance spectrum for which they predict characteristic features. 1.3.2. Mean-field results: Ginzburg–Landau approach While the solution of the full quasiclassical equations in the full δµ and T range could be solved only for stripe textures, more insight can be gained in restricted regions of the phase diagram. In the vicinity of the second-order transition from the normal to the superconducting phase a (generalized) Ginzburg–Landau expansion of the free energy in terms of the superconducting order parameter were derived from the microscopic theory. The central focus of these studies is “pattern formation” associated with the higher-order terms contributions. The latter lift the degeneracy of the primary plane-wave order parameters ∼ eiqm ·R and induce higher-harmonics. Neglecting the admixture of higher harmonics, Larkin and Ovchinnikov2 compared three cases, i.e., the single-vector state discussed in the previous section, the striped phase, and the simple cubic crystal and concluded that among these candidates the striped phase has the lowest energy. Shimahara predicts a series of phase transitions between different periodic structures as shown in Fig. 1.5. Recently, a detailed study was presented by Bowers and Rajagopal37 who analyzed 23 different crystalline structures. The coefficients of the free-energy functional derived from the microscopic Gorkov equations29 allow for a determination of the stable structures within weak-coupling theory. The name of the multiple-wave configurations refers to the polyhedron inscribed in a sphere of radius |q| whose BCS50FFLO 4:39 World Scientific Review Volume - 9.75in x 6.5in Breaking Translational Invariance by Population Imbalance BCS50FFLO 15 hexagonal triangular 1 1D / 0 square B Hc2 June 30, 2010 0.5 + + (T ,H ) BCS (uniform) 0 0 0.5 1 T / Tc Fig. 1.5. Phase diagram of an s-wave superconductor with cylindrical Fermi surface.3 The chemical-potential mismatch δµ = gµB H is due to the Zeeman splitting of the quasiparticle states in a magnetic field applied perpendicular to the axis of the Fermi-surface cylinder. With decreasing temperature several types of periodic structures are predicted in the FFLO state. vertices correspond to the wave vectors qm . Among the structures which are stable within sixth-order expansion the octahedron gives the lowest free energy. Special attention should be paid to the cube structure for which the coefficients of the quadratic, quartic, and sextic term in the GL expansion are negative. In real space, ∆(R) exhibits a periodic face-centered cubic structure. These candidate states are displayed schematically in Fig. 1.6. To actually discuss the free-energy one has to go to the eighth order. Bowers and Rajagopal argue that this structure might correspond to a rather low value of the free energy.37 1.3.3. Fluctuations Having discussed the mean-field predictions we next turn to the superconducting fluctuations. In this context we have to distinguish between the thermal fluctuations at finite temperatures T > 0 and the T = 0 quantum fluctuations. While the former are predominantly classical the dynamic nature of the latter is essential. Thermal fluctuations in superconductors have been studied for a long time. For a review see Ref. 38. The role of phase fluctuations of the modulated order parameter is most prominent in isotropic systems where the FFLO states are infinitely degenerate. The situation is different in the so-called “generic” case where the degeneracy manifold is reduced to isolated points in momentum space either by anisotropies in the normal-state quasiparticle properties or the node structure of June 30, 2010 4:39 World Scientific Review Volume - 9.75in x 6.5in 16 -1 Gertrud Zwicknagl and Jochen Wosnitza 0 1 Fig. 1.6. Unit cell of candidate crystalline FFLO states in isotropic 3D superconductors. The octahedron state (left panel) gives the lowest energy within sixth-order Ginzburg–Landau expansion. Qualitative considerations suggest that the cube structure (right panel) should be the most favorable structure. The contours correspond to √ ∆(R)/∆max = −0.9, −0.5, −0.3, 0, 0.3, 0.5, 0.9. The lengths of the cubes are 2π/ |q| and 2π/ |q| 3 for the octahedron and the cube structure, respectively. the superconducting order parameter. Quantum fluctuations at T = 0 have received little attention. Samokhin and Marenko39 calculated the corrections to the spin susceptibility and the quasiparticledecay rate of fermionic quasiparticles for both the isotropic and the generic case. The results reflect the singular behavior of the mean-field ground-state energy displayed in Fig. 1.3. Diener et al. find Fermi-liquid interaction corrections to thermodynamic properties as a consequence of quantum fluctuations.40 1.3.4. Microscopic studies Microscopic model studies beyond the mean-field approximation have been performed for quasi-1D systems. The exact ground states of two-component Fermi liquids with attractive contact interaction and unequal densities are known from Bethe ansatz. Three phases appear at T = 0: The paired superfluid state, the polarized normal Fermi liquid and an intermediate partially polarized phase which exhibits FFLO-type correlations. These findings were recently confirmed by accurate Density Matrix Renormalization Group (DMRG) and Quantum Monte Carlo (QMC) calculations (see Refs. 41–44 and references therein). In the weak-coupling limit the phase diagram is well described by mean-field theory. BCS50FFLO June 30, 2010 4:39 World Scientific Review Volume - 9.75in x 6.5in Breaking Translational Invariance by Population Imbalance BCS50FFLO 17 1.4. Search for experimental realization Shortly after the theoretical predictions for the possible existence of an inhomogeneous superconducting state at high magnetic fields and low temperatures first experimental searches started. It took, however, more than 30 years until first claims for the observation of the FFLO state appeared. Yet, those proved to be not well founded. Only in the last decade better justified evidences have been reported for homogeneous materials (heavy-fermion and organic superconductors) as well as for heterogeneous materials (artificial superlattices). 1.4.1. Homogeneous materials In real superconducting materials two main conditions have to be fulfilled in order to allow the FFLO state to occur. First, the orbital critical field, √ Horb , should be sufficiently larger than the Pauli-paramagnetic limit, HP = ∆0 /( 2µB ), where ∆0 is the superconducting energy gap at T = 0. Or more precise, the Maki parame√ ter,45 α = 2Horb /HP , should be larger than 1.8.46 Second, the superconductor needs to be in the clean limit with a mean-free path, `, much larger than the coherence length ξ. These are rather rigorous conditions that are not satisfied by many superconductors. Likely candidates for a possible realization of the FFLO state are heavy-fermion or layered superconductors. In heavy-fermion materials the high effective mass, mef f , results in a small Fermi velocity, vF , which in turn leads to a short coherence length (ξ ∝ vF ) and, consequently, a large orbital critical field. With ` in high-quality heavy-fermion crystals much larger than ξ, the FFLO state may well be expected. Layered, or quasi-two-dimensional superconductors, such as some cuprates, many organic superconductors, or artificial superlattices may be even better suited for exhibiting the FFLO state.3,6 For such materials the orbital pair breaking can be greatly suppressed when applying the magnetic field parallel to the superconducting layers. At the same time, samples of very high quality are available with sufficiently large mean-free paths. Nevertheless, even up to now only very few condensed-matter realizations exist that are reported to show indications for an FFLO-like state. First reports appeared in the 1990s, in which evidence for such an inhomogeneous state was suggested to exist in the heavy-fermion compounds UPd2 Al3 ,47 CeRu2 ,48 and UBe13 .49 These claims, however, later had to be revised or are inconclusive. See Refs. 3, 6, and 50 for more details. In the first decade of the 21st century new experimental work strongly suggested the existence of an FFLO state in novel superconducting materials. These are the heavy-fermion compound CeCoIn5 51,52 and the quasi-two-dimensional organic superconductors. Whereas for CeCoIn5 some recent experimental results53 cast some doubt on the genuine realization of the FFLO state, the organic materials make a strong case in favor for such a state. In the following, the experimental status quo for these materials will be discussed in more detail. 4:39 World Scientific Review Volume - 9.75in x 6.5in 18 BCS50FFLO Gertrud Zwicknagl and Jochen Wosnitza 1.4.1.1. Heavy-fermion systems A recent prime candidate for the realization of an FFLO state is CeCoIn5 . It is a heavy-fermion superconductor with Tc = 2.3 K and tetragonal crystal structure.54 It is a clean type-II superconductor with a large orbital critical field, a sufficiently large Maki parameter, and an unusual field-temperature phase diagram.51,52,55 Therefore, all conditions to observe the FFLO state are fulfilled. And indeed, specific-heat data51,52 as well as thermal-conductivity56 and penetrationdepth measurements using a self-resonant tank circuit57 showed clear evidence for a phase transition within the superconducting state, as expected for the FLLO state. 11.4 2 C/T (J/mol K ) 2 0 11.2 12 1.2 T2 0.75 1.3 11 0.3 1.5 10.8 10.6 0.4 10 T (K) 8 2 6 1.0 11.0 11.2 0.2 0.50 11.4 1.0 3 2 C (J/mol K ) H (T) || [110] 2.0 2.5 H (T) 4 (C-CSch)/T (J/mol K ) June 30, 2010 Tc T2 10.6 3.0 3.8 5.0 10.4 10.2 1 10.0 0 0.0 0.4 0.8 1.2 T (K) 1.6 2.0 2.4 9.8 0.0 0.2 0.4 0.6 0.8 1.0 1.2 T (K) Fig. 1.7. (left panel) Specific heat of CeCoIn5 in magnetic fields aligned parallel to the [110] direction. A Schottky-like nuclear contribution has been subtracted. The inset show the anomalies, T2 (originally called TF F LO ), at 10.6 and 11 T. (right panel) Contour plot of the electronic part of the specific heat divided by temperature for H || [110]. The grey lines denote Tc and T2 . After Ref. 51. The specific-heat data of Bianchi et al.51 for magnetic fields aligned along the [110] direction is shown in the left panel of Fig. 1.7. First of all, above about 10 T and below about 1 K, the phase transition from the normal into the superconducting state changes from second to first order. This can be realized by the pronounced sharpening of the anomalies as well as by the occurrence of hysteresis in the specific-heat data collected by use of the relaxation method for rising and falling temperatures. Further to that, a small but clear anomaly is resolved at lower temperatures around 300 mK, labeled T2 (originally labeled TF F LO ) in the inset of Fig. 1.7. This anomaly is most prominent for in-plane field orientations, but a smaller anomaly was found as well for the field aligned along the c axis.51 The phase diagram over a narrow region in field and temperature is shown in the right panel of Fig. 1.7 as a contour plot. The data were collected by use of the relaxation method.51 Besides the phase transition from the normal to the superconducting state at Tc , a second phase transition at low temperatures and high fields within the superconducting region is clearly evident (T2 ). Such kind of phase diagram, confirmed by other methods as well, is very suggestive for an FFLO state. June 30, 2010 4:39 World Scientific Review Volume - 9.75in x 6.5in Breaking Translational Invariance by Population Imbalance BCS50FFLO 19 There are, however, some features in contrast to the expected behavior. Especially, there is no saturation of the upper critical field, Hc2 , due to the Pauli limiting observed and there is no upturn of Hc2 at low temperatures at which the additional phase appears. In order to get a definitive proof for the existence of an FFLO state, the spatial modulation of the superconducting order parameter should be measured. The method of choice for that purpose is small-angle neutron scattering. By that, the expected periodic oscillation of the magnetic-field strength along the applied field may in principle be detected. Indeed, in 2008 Kenzelmann et al. used high-field neutron diffraction to search for the magnetic response of CeCoIn5 in the suggested FFLO phase.53 Clear evidence of magnetic Bragg peaks with an incommensurate ordering vector Q = (q, q, 0.5) was found. This Bragg peaks are not present outside, what is now called, the Q phase. In the FFLO state, one would expect the Cooper pairs to carry a momentum that depends on the magnetic field via |q| = 2µB H/(~vF ). In the experiment, however, q = 0.442 was found to be independent of the magnetic field.53 This is in stark contradiction to the usual picture of an FFLO state. Anyway, the finding that antiferromagnetism appears only inside the superconducting state of CeCoIn5 at high fields and low temperatures is remarkable. It strongly suggests that the superconducting condensate carries a field-independent momentum. A similar behavior seems to occur for magnetic fields applied parallel to the c direction. Recent µSR data hint to a field-induced coupled superconducting and spin-density-wave order for this field orientation.58 The findings of Kenzelmann et al.53 have triggered numerous theoretical efforts trying to explain the nature of the highly unusual Q state. Recently, Mierzejewski et al. discussed the possibility of a mutual enhancement of an incommensurate magnetic order and FFLO superconductivity.59 Before that, Yanase and Sigrist suggested that the observed antiferromagnetism might be stabilized by the FFLO state.60 On the basis of Bogoliubov–de Gennes equations this was argued to be caused by the appearance of Andreev bound states localized around the zeros of the FFLO order parameter. With other words, the antiferromagnetic order should occur in regions where the superconducting order parameter vanishes, as opposed to Ref. 59 where the two orders mutually enhance each other. Anyway, in both cases the antiferromagnetic order might occur in the FFLO state even when it is neither stable in the normal state nor in the BCS state. In agreement with this prediction, recent nuclear magnetic resonance (NMR) experiments indicated that the incommensurate magnetic order in CeCoIn5 is likely to coexist with a modulated superconducting phase, that may well be the FFLO state.61 The authors further found some indication for a new region below the Q phase in the phase diagram, which could be an FFLO phase without magnetic order. It is evident that further work is necessary to settle all the open issues in this highly fascinating material. 4:39 World Scientific Review Volume - 9.75in x 6.5in 20 BCS50FFLO Gertrud Zwicknagl and Jochen Wosnitza 1.4.1.2. Organic superconductors Besides the heavy-fermion materials, the quasi-two-dimensional (2D) organic superconductors are prime candidates for exhibiting the FFLO state. When applying the magnetic field exactly parallel to the highly conducting planes the orbital critical field will be greatly enhanced. In a number of different experiments some indications for an FFLO state have been reported. In most of the experiments, however, no thermodynamic proof was given. Only recently, clear thermodynamic evidence for a narrow intermediate superconducting state was presented.62 One of the first reports claiming evidence for an FFLO state in a 2D organic superconductor was presented for κ-(BEDT-TTF)2 Cu(NCS)2 , where BEDT-TTF is bisethylenedithio-tetrathiafulvalene. This conclusion was based on measurements sensitive to the loss in vortex stiffness.63 The observed rather broad features in the signal and the derived phase diagram are, however, largely at odd with the thermodynamic evidences for this material presented below. 0 1 2 13 12 #6 11 0.15 10 µ0Hc2 (T) #1 -1 -2 κ/T(Wm K ) + offset June 30, 2010 #2 0.10 10 9 5 #5 0.05 8 10 12 14 Magnetic field (T) 16 0 0 2 4 6 Temperature (K) Fig. 1.8. (left) Field dependence of the thermal conductivity of four different λ-(BETS)2 GaCl4 samples at 0.3 K. The field was aligned parallel to the conducting layers. The curves for sample 6 and 5 are shifted up and down by 0.04 Wm−1 K−2 , respectively. (right) Phase diagram for sample 2. Up and down triangles are from the resistive transitions for parallel and perpendicular field orientations, respectively. Open circles are from thermal conductivity. The inset shows the lowtemperature part of the phase diagram for sample 1 (closed circles) and sample 2 (open circles), respectively. The diamonds are from the low-field slope change in κ/T (left arrows in the left panel) for sample 1. After Ref. 64. For another 2D organic superconductor, λ-(BETS)2 GaCl4 , where BETS is bisethylenedithio-tetraselenafulvalene, thermal-conductivity, κ, data indicate a possible FFLO state.64 Tanatar et al. investigated samples of different quality, which was determined by the resistivity ratio or by the relative thermal-conductivity maximum. For low-quality samples (2 and 5 in Fig. 1.8), the rather sharp increase of κ/T June 30, 2010 4:39 World Scientific Review Volume - 9.75in x 6.5in Breaking Translational Invariance by Population Imbalance BCS50FFLO 21 at Hc2 might indicate a broadened first-order transition. For high-quality samples (1 and 6 in Fig. 1.8), this feature is replaced by two distinct slope changes that are much farther apart than in the low-quality samples. The magnetic phase diagram for samples 1 and 2 are shown in the right panel of Fig. 1.8. For sample 2, a clear saturation of Hc2 is observed below about 1 K, probably due to the Pauli-limiting effect. For the high-quality sample 1, the Hc2 line continues to grow even below 1 K (inset of Fig. 1.8). When interpreting the low-field slope change as another phase transition (diamonds in the inset of Fig. 1.8), a phase diagram as expected for a superconductor with an FFLO state evolves. Although these experimental results give no definite proof for such an inhomogeneous state in this organic superconductor, all observed features are in accord with such a conclusion. Another isostructural material, λ-(BETS)2 FeCl4 , where just gallium is replaced by magnetic iron, has become famous because of its field-induced superconducting state.65,66 Thereby, after removing a zero-field antiferromagnetic state by the application of an in-plane magnetic field, superconductivity appears in the field range between 17 and 45 T. This behavior is well understood by the Jaccarino– Peter compensation mechanism.67 Thereby, the internal exchange field of the iron atoms acting on the π electrons of the BETS molecules becomes compensated in the applied external field. Fig. 1.9. Phase diagram of λ-(BETS)2 FeCl4 for a magnetic field aligned parallel to the conducting layers (H||c). The triangles depict the transition from the antiferromagnetic-insulating (AFI) to the paramagnetic (PM) state, solid circles correspond to the onset of superconductivity, Hc2 , and open circles are extracted from the dip positions in the second derivative of the resistance (solid arrows in the inset). The squares show estimated values of the order-parameter wavelength in the assumed FFLO states at T = 0.7 K (see text). The solid lines are guides to the eye. The dotted arrows in the inset correspond to broader features at Hc2 . After Ref. 68. Since λ-(BETS)2 FeCl4 is a clean-limit superconductor, as evidenced by the observation of magnetic quantum oscillations, and the Pauli limit is estimated at 4:39 World Scientific Review Volume - 9.75in x 6.5in 22 BCS50FFLO Gertrud Zwicknagl and Jochen Wosnitza 13 T,68 the FFLO state may be expected. When Uji et al. measured the interplane resistance for in-plane fields, anomalous dip structures were observed.68 These features appear much clearer in the second derivative of the field-dependent resistance curves (inset of Fig. 1.9) which allowed to construct the phase diagram shown in Fig. 1.9. The Jaccarino–Peter compensation field is about 32 T. Therefore, critical fields appear both below as well as above this value with two regions for possible FFLO states. The multiple dip structures observed are suggested to be caused by a commensurability effect.68 According to Bulaevskii et al. a possible Josephsonvortex lattice (with lattice constant l) may get pinned at the oscillating FFLO order parameter (with wavelength λF F LO ).69 This effect may lead to the observed dip structures whenever m = l/λF F LO becomes an integer. Whether this assumption is correct requires further studies. Another recent report suggested a possible FFLO state in the 2D organic superconductor β 00 -(BEDT-TTF)2 SF5 CH2 CF2 SO3 .70 This was based on in-plane penetration-depth measurements by using a tunnel-diode-oscillator technique. Some features in the second derivative of the observed frequency changes were attributed to transitions into the FFLO phase and to Hc2 . Below about 1.23 K, Hc2 exceeds the Pauli-limiting field and the Hc2 line becomes steeper. At the same time the second feature at lower fields suggests an emerging FFLO state.70 The resulting phase diagram needs, however, further support. Further to that, there has recently been a report suggesting an FFLO state in the quasi-one-dimensional organic superconductor (TMTSF)2 ClO4 , where TMTSF stands for tetramethyltetraselenafulvalene.71 Constructing the magnetic phase diagrams from resistivity measurements, one low-quality sample revealed a saturation of Hc2 reminiscent of Pauli limiting, whereas a better-quality sample showed a clear upturn in Hc2 at lowest temperatures. The resulting Hc2 data are very similar to the phase diagrams shown in Fig. 1.8 here for λ-(BETS)2 GaCl4 .64 2.0 H (T) H (T) || planes 80 0 21.5 20 22 -2 (mJ mol -1 21.5 22 1.0 22.5 22 T 80 60 23 24 40 28 2.4 2.6 2.8 3.0 40 C /T 23 22.5 60 -1 -2 K ) 21 100 21 K ) 1.5 25 e C/T (J mol June 30, 2010 0.5 20 -(BEDT-TTF) Cu(NCS) (a) 0.0 0 2 2 4 6 T (K) 8 (b) 2 10 12 2.0 2.5 3.0 3.5 4.0 T (K) Fig. 1.10. (a) Temperature dependence of the specific heat divided by temperature, C/T , of κ(BEDT-TTF)2 Cu(NCS)2 for magnetic fields applied parallel to the superconducting layers. (b) Low-temperature part of the electronic part of the specific heat, Ce /T . Data taken in 14 T applied perpendicular to the layers were used to separate the phonon contribution. See Ref. 62 for more details. 4:39 World Scientific Review Volume - 9.75in x 6.5in BCS50FFLO Breaking Translational Invariance by Population Imbalance 23 In all of the above cases no thermodynamic proof for an FFLO state in organic superconductors was given. Only for κ-(BEDT-TTF)2 Cu(NCS)2 such evidence has been presented recently.62 For magnetic fields aligned exactly parallel to the 2D layers spike-like anomalies in the specific heat are observed for fields above 21 T and temperatures below 3 K [Fig. 1.10(a)]. These features can be much better resolved after subtraction of the phonon contribution to the specific heat. For that, data in the normal state measured at 14 T applied perpendicular to the layers have been used.62 The resulting electronic contribution to the specific heat, Ce , divided by temperature is shown in Fig. 1.10(b). At about 21 T, a sharpening of the specific-heat anomaly and at 21.5 T a spike in Ce occurs. This is clear evidence for a first-order nature of the phase transition from the normal into the superconducting state. For higher fields, a second very sharp anomaly appears within the superconducting state. This proves the existence of an additional thermodynamic phase. The transition at lower temperatures shows a well-resolvable hysteresis, while the main superconducting transition reveals a smaller hysteresis [inset of Fig. 1.10(b)]. Above 23 T the transition left the temperature window accessible in the experiment.62 25 κ-(BEDT-TTF)2Cu(NCS)2 20 15 23 H (T) June 30, 2010 10 Hc2 TFFLO up TFFLO dn 22 21 5 20 2 0 0 3 2 4 4 5 6 8 10 T (K) Fig. 1.11. Phase diagram of κ-(BEDT-TTF)2 Cu(NCS)2 for fields applied parallel to the superconducting layers. The solid line represents the calculated Hc2 using the known band-structure parameters. After Ref. 62. From these data the magnetic phase diagram shown in Fig. 1.11 was extracted. From the very steep initial increase of Hc2 an orbital critical field of roughly 130 T can be estimated. This large value results from the strongly reduced orbital currents for the field orientation parallel to the layers. Towards higher fields, however, Hc2 levels off towards saturation at lower temperatures. This clearly signals the crossover to Pauli-paramagnetic limitation. The Pauli limit, HP , can be determined quite accurately from the known gap value, ∆0 , extracted in earlier specific-heat studies.72,73 Using ∆0 /kB Tc = 2.4,73 leads to HP = 23 T which fits nicely with the 4:39 World Scientific Review Volume - 9.75in x 6.5in 24 BCS50FFLO Gertrud Zwicknagl and Jochen Wosnitza field of ∼ 21 T where the sharp first-order phase transition emerges [Fig. 1.10(b)]. Above this field, the curvature of the Hc2 line clearly changes. Together with an increased slope of this line, the second phase transition appears. This is favorably in line with the expectations for the existence of an FFLO state. A comparison with the calculated phase diagram is shown by the solid line in Fig. 1.11. For that, the well-known electronic band-structure parameters of κ-(BEDT-TTF)2 Cu(NCS)2 have been considered and s-wave superconductivity has been assumed.72–74 The latter, however, is not an essential ingredient. The calculated line and the experimental data agree very well except at lower temperatures. This as well as the unexpected small area of the FFLO phase may be caused by a small misalignment of the sample in the experiment. Also, the theoretical description might be improved when taking more detailed information on the electronic parameters into account. For the 2D organic superconductors based on BEDT-TTF further evidence for the existence of the FFLO state has been gathered. For κ-(BEDT-TTF)2 Cu(NCS)2 , the results from magnetic-torque studies are shown in Fig. 1.12.75 With decreasing temperature the magnetic torque, which is proportional to the magnetization, shows an increasingly sharp transition at Hc2 . This indicates that the Pauli limit, HP , is reached. Nevertheless, superconductivity survives even beyond this field for lower temperatures. In addition, a second sharp feature appears in the torque signal below Hc2 , signalling the evolution of the FFLO phase. The magnetic phase diagram constructed from the torque data is shown in the right panel of Fig. 1.12.75 These results nicely confirm the specific-heat data for the Hc2 line. There is, however, a discrepancy in the extension of the FFLO phase. This might be explained by the much better in-plane alignment of the magnetic field in the torque measurements which was made possible by an in-situ rotation of the torque platform. The alignment in the specific-heat experiment is estimated to be not better than about (a) FFLO phase HFFLO (b) Pauli limit 5.4 K 25 20 15 2.9 K 8 K 4.2 K 10 1.7 K H (T) Normalized torque signal June 30, 2010 Hc2 HFFLO 8 12 16 20 H (T) 24 28 2 4 6 5 8 0 10 T (K) Fig. 1.12. (a) Field dependence of the magnetic-torque signal of κ-(BEDT-TTF)2 Cu(NCS)2 for in-plane magnetic fields at different temperatures. (b) Magnetic phase diagram constructed from the data. After Ref. 75. June 30, 2010 4:39 World Scientific Review Volume - 9.75in x 6.5in Breaking Translational Invariance by Population Imbalance BCS50FFLO 25 1 deg. 1.4.2. Heterogenous systems Besides the still partially controversial evidences for the FFLO state in the homogeneous systems, a quasi-one-dimensional FFLO-like state may exist in artificially layered superconducting/ferromagnetic superlattices.76 Due to the proximity effect Cooper pairs from the superconductor can enter the ferromagnetic region. In the spin-split bands of the ferromagnet, however, the wavevectors of the spin-up and spin-down electrons must be largely different resulting in a Cooper pair with finite momentum.77 Consequently, the real-space pairing function oscillates spatially inside the ferromagnet. Of course, on top of that oscillation the pairing function decays rapidly inside the ferromagnet. However, if the ferromagnetic layer is thin enough, the pairing-function wave may be reflected at the opposite ferromagneticlayer surface, similar as in a Fabry–Pérot interferometer. Upon changing the ferromagnetic layer thickness, dF , the pairing functions running oppositely may interfere either constructive or destructive. This eventually may lead to an oscillatory proximity effect, i.e., Tc might oscillate as function of dF .78,79 For optimum parameters this could even result in a reentrant superconductivity. A first report on the observation of reentrant superconductivity in Fe/V/Fe trilayers as a function of the iron thickness was given in Ref. 80. The Tc oscillation length is given by the magnetic coherence length ξF O = ~vF /Eex , where Eex is the exchange-splitting energy. For the strong ferromagnet iron this length scale is very short (0.7 − 1.0 nm). Indeed, superconductivity in the Fe/V/Fe system vanished at this iron-layer thickness, but the number of experimental points is low and shows a large scatter.80 A much clearer evidence for such a reentrant behavior has been given by Zdravkov et al. for the bilayer system Nb/Cu1−x Nix .81 Alloying the strong ferromagnet nickel by copper reduces Eex strongly which led to ξF O = 8.6 nm for the chosen Cu41 Ni59 layer. This largely reduces the influence of surface roughness on the interference effects. The thicknesses of the superconducting niobium layers were chosen so that Tc was in the right range to be strongly susceptible on the thickness of the Cu41 Ni59 layer, dCuNi (inset of Fig. 1.13). In order to produce samples with different dCuNi , but exactly the same niobium thickness a wedge-shape ferromagnetic Cu41 Ni59 layer was deposited on top of the niobium layer (right panel of Fig. 1.13). After evaporation of a silicon cap layer, samples of equal width were cut perpendicular to the wedge.81 The resistively determined Tc s as a function of dCuNi for two different niobium layer thicknesses are shown in the left panel of Fig. 1.13. For the thicker niobium layer a clear minimum in Tc is resolved. For the 7.3 nm thick niobium layer, Tc vanishes at dCuNi ≈ 5 nm and reappears at about 12 nm. The data can be well described using a model for a clean ferromagnet, i.e., a ferromagnet where the electronic mean-free path is larger than ξF O (solid lines in Fig. 1.13.82,83 Consequently, superconducting/ferromagnetic superlattices seem to be a June 30, 2010 4:39 26 World Scientific Review Volume - 9.75in x 6.5in Gertrud Zwicknagl and Jochen Wosnitza Fig. 1.13. (left) Critical temperature, Tc , of an (a) 8.3 and (b) 7.3 nm thick niobium layer as a function of the thickness of a ferromagnetic Cu41 Ni59 layer. The solid and dashed lines are calculations for the clean and dirty cases, respectively. The inset shows Tc as a function of niobium-layer thickness for a 56 nm thick Cu41 Ni59 layer with the solid line calculated for the clean case. (right) Sketch of the investigated superconductor-ferromagnet bilayer. After Ref. 81. good realization for studying FFLO-like behavior. 1.5. Summary and Outlook The central focus of the present work are the Fulde-Ferrell-Larkin-Ovchinnikov states which, in addition to off-diagonal long-range order break spatial symmetries. These superfluid phases are suggested by mean-field analyses to occur at low temperatures in multi-component fermionic superfluids with population imbalance. The theoretical considerations apply to a wide variety of systems including metals, ultra-cold atoms, nuclear matter, and dense quark systems. The discussion presented here refers to the weakly interacting BCS regime where the systems mentioned are all described by essentially the same microscopic theory. This fact implies that the knowledge and insights gained by studying superconducting metals in high magnetic fields or ultra-cold atoms can provide explanations for phenomena observed in nuclear or astrophysical contexts. There are indications that FFLO phases are realized in some highly anisotropic superconductors. Especially, for the low-dimensional organic superconductors a number of experimental facts point to the existence of such an inhomogeneous state, whereas the situation is much more controversial for heavy-fermion materials. The main criteria employed to identify perspective candidate systems have been the upturn of the Pauli-limited critical field and the appearance of a firstorder transition from the normal to the superconducting state at low temperatures BCS50FFLO June 30, 2010 4:39 World Scientific Review Volume - 9.75in x 6.5in Breaking Translational Invariance by Population Imbalance BCS50FFLO 27 as well as the existence of transitions within the superconducting phase. Besides for these homogeneous systems, FFLO-like behavior may exist in artificial superconducting/ferromagnetic superlattices that show an oscillating or even reentrant superconducting phase transition as a function of the ferromagnetic layer thickness. An unambiguous identification of FFLO states requires a better qualitative understanding of superfluids with periodically textured order parameters. The investigations should concentrate on characteristic features which are tied to the quantum nature of the order parameter and reflect its periodicity. Prominent candidates are Andreev bound-states which should form bands in a superconductor with a periodically modulated order parameter. The spatial variation of the latter should give rise to characteristic van Hove-type structures in the corresponding spectral density. The latter can be observed by tunneling spectroscopy. In addition, it should affect transport properties. The interpretation of experimental data needs detailed quantitative reference calculations which account for realistic quasiparticle dispersion and include quasiparticle interactions. An appropriate theoretical treatment will require new effective calculational tools. In particular, it is highly desirable to have methods which allow for direct “unbiased” minimization of the free energy. Finally, the role of (quantum) fluctuations should be considered. We hope that this article will stimulate further work on the exciting subject of fermionic superfluids with population imbalance and the FFLO phases. Acknowledgments We have benefitted from discussions with many colleagues, especially we would like to thank P. Fulde, R. Lortz, A. D. Bianchi, B. Bergk, G. Eilenberger, M. Sigrist, L. N. Bulaevskii, M. R. Beasley, and D. J. Scalapino for stimulating discussions. GZ acknowledges the hospitality of the Kavli Institute for Theoretical Physics where part of the manuscript was completed. This work was supported in part by the National Science foundation under Grant No. PHY05-51164 and by EuroMagNET (EU contract No. 228043) References 1. 2. 3. 4. 5. 6. 7. 8. 9. P. Fulde and R. A. Ferrell Phys. Rev. 135, A550, (1964). A. I. Larkin, , and Y. N. Ovchinnikov, JETP (U. S. S. R.). 47, 1136, (1964). Y. Matsuda and H. Shimahara, J. Phys. Soc. Jpn. 76, 051005, (2007). A. I. Buzdin, Proximity effects in superconductor-ferromagnet heterostructures, Rev. Mod. Phys. 77(3), 935–976 (Sep, 2005). doi: 10.1103/RevModPhys.77.935. D. E. Sheehy and L. Radzihovsky, Annals of Physics. 322, 1790–1924, (2007). R. Casalbuoni and G. Nardulli, Rev. Mod. Phys. 76, 263, (2004). B. S. Chandrasekhar, Appl. Phys. Lett. 1, 7, (1962). A. M. Clogston, Phys. Rev. Lett. 9, 266, (1962). G. Sarma, J. Phys. Chem. Solids. 24, 1029, (1963). June 30, 2010 4:39 28 World Scientific Review Volume - 9.75in x 6.5in Gertrud Zwicknagl and Jochen Wosnitza 10. D. Saint-James, D. Sarma, and E. J. Thomas, Type II Superconductivity. (Pergamon, New York, 1969). 11. G. E, W. V. Liu, and F. Wilczek, Phys. Rev. Lett. 91, 032001, (2003). 12. A. A. Abrikosov, Zh. Eksp. Teor. Fiz. 32, 1442, (1957). 13. K. Maki, Phys. Rev B. 148, 362, (1966). 14. P. Fulde, Adv. Phys. 22, 667, (1973). 15. V. P. Mineev and K. V. Samokhin, Introduction to Unconventional Superconductivity. (Gordon and Breach Science Publishers, 1999). 16. G. Eilenberger in Supraleitung und verwandte Quantenphänomene, Kernforschungsanlage Jülich, Ferienkurs, (1988). 17. J. Bardeen, L. N. Cooper, and J. R. Schrieffer, Phys. Rev. 108, 1175, (1957). 18. J. Bardeen, Rev. Mod. Phys. 34, 667, (1962). 19. G. Zwicknagl and P. Fulde, Z. Phys. 43, 23, (1981). 20. P. Fulde and G. Zwicknagl, J. Appl. Phys. 53, 8064, (1982). 21. W. Baltensperger and S. Straessler, Phys. Kondens. Materie. 1, 20, (1963). 22. R. Combescot and C. Mora, Phys. Rev B. 71, 144517, (2005). 23. K. Maki and H. Won, Czech. J. Phys. 46, 1035, (1996). 24. G. Eilenberger, Z. Phys. 214, 195, (1968). 25. A. I. Larkin and Y. N. Ovchinnikov, Zh. Eksp. Teor. Fiz. 55, 2262, (1968). 26. G. M. Eliashberg, Soviet Physics JETP. 34, 668, (1972). 27. P. G. deGennes, Rev. Mod. Phys. 36, 225, (1964). 28. Y. Nambu, Phys. Rev. 117, 648, (1960). 29. L. P. Gorkov, Zh. Eksp. Teor. Fiz. 36, 1918, (1959). 30. J. W. Serene and D. Rainer. 101, 221, (1983). 31. H. Burkhardt and D. Rainer, Ann. Phys. 3, 181, (1994). 32. S. Matsuo, S. Higashitani, Y. Nagato, and K. Nagai, J. Phys. Soc. Jpn. 67, 280, (1998). 33. A. B. Vorontsov, J. A. Sauls, and M. J. Graf, Phys. Rev B. 72, 184501, (2005). 34. H. Shimahara, J. Phys. Soc. Jpn. 67, 1872, (1998). 35. H. Shimahara and D. Rainer, J. Phys. Soc. Jpn. 66, 3591, (1997). 36. K. Yang and S. L. Sondhi, Phys. Rev B. 57, 8566, (1998). 37. J. A. Bowers and K. Rajagopal, Phys. Rev. D. 66, 065002, (2002). 38. A. I. Larkin and A. A. Varlamov, in Superconductivity, Vol. I, ed. by K. H. Bennemann and J. B. Ketterson, p. 369. Springer, Berlin. 39. K. V. Samokhin and M. S. Mar’enko, Phys. Rev. B. 73, 144502, (2006). 40. R. B. Diener, R. Sensarma, and M. Randeria, Phys. Rev. A. 77, 023626, (2008). 41. A. Feiguin and F. Heidrich-Meisner, Phys. Rev. B. 76, 220508(R), (2007). 42. A. E. Feiguin and D. A. Huse, Phys. Rev. B. 79, 100507(R), (2009). 43. G. G. Batrouni, M. H. Huntley, V. G. Rousseau, and R. T. Scalettar, Phys. Rev. Lett. 100, 116405, (2008). 44. M. Casula, D. M. Ceperley, and E. J. Mueller, Phys. Rev. A. 78, 033607, (2008). 45. K. Maki and T. Tsuneto, Prog. Theor. Phys. 31, 945, (1964). 46. L. W. Gruenberg and L. Gunther,Phys. Rev. Lett. 16, 996, (1966). 47. K. Gloos, R. Modler, H. Schimanski, C. D. Bredl, C. Geibel, F. Steglich, A. I. Buzdin, N. Sato, and T. Komatsubara, Phys. Rev. Lett. 70, 501, (1993). 48. A. D. Huxley, C. Paulsen, O. Laborde, J. L. Tholence, D. Sanchez, A. Junod, and R. Calemczuk, J. Phys.: Condens. Matter. 5, 7709, (1993). 49. F. Thomas, B. Wand, T. Lühmann, P. Gegenwart, G. R. Stewart, F. Steglich, J. P. Brison, A. Buzdin, L. Glémot, and J. Flouquet, J. Low Temp. Phys. 102, 117, (1996). 50. A. Bianchi, R. Movshovich, N. Oeschler, P. Gegenwart, F. Steglich, J. D. Thompson, BCS50FFLO June 30, 2010 4:39 World Scientific Review Volume - 9.75in x 6.5in Breaking Translational Invariance by Population Imbalance BCS50FFLO 29 P. Pagliuso, and J. L. Sarrao, Phys. Rev. Lett. (137002), (2002). 51. A. Bianchi, R. Movshovich, C. Capan, P. Pagliuso, and J. Sarrao, Phys. Rev. Lett. 91, 187004, (2003). 52. H. A. Radovan, N. A. Fortune, T. P. Murphy, S. T. Hannahs, E. C. Palm, S. W. Tozer, and D. Hall, Nature. 425, 51, (2003). 53. M. Kenzelmann, T. Strässle, C. Niedermayer, M. Sigrist, B. Padmanabhan, M. Zolliker, A. D. Bianchi, R. Movshovich, E. D. Bauer, J. L. Sarrao, and J. D. Thompson, Science. 321, 1652, (2008). 54. C. Petrovic, P. G. Pagliuso, M. F. Hundley, R. Movshovich, J. L. Sarrao, J. D. Thompson, Z. Fisk, and P. Monthoux, J. Phys.: Condens. Matter. 13, L337, (2001). 55. A. D. Bianchi, M. Kenzelmann, L. DeBeer-Schmitt, J. S. White, E. M. Forgan, J. Mesot, M. Zolliker, J. Kohlbrecher, R. Movshovich, E. D. Bauer, J. L. Sarrao, Z. Fisk, C. Petrović, and M. R. Eskildsen, Science. 319, 177, (2008). 56. C. Capan, A. Bianchi, R. Movshovich, A. D. Christianson, A. Malinowski, M. F. Hundley, A. Lacerda, P. G. Pagliuso, and J. L. Sarrao, Phys. Rev. B. 70, 134513, (2004). 57. C. Martin, C. C. Agosta, S. W. Tozer, H. A. Radovan, E. C. Palm, T. P. Murphy, and J. L. Sarrao, Phys. Rev. B. 71, 020503, (2005). 58. J. Spehling, R. H. Heffner, J. E. Sonier, N. Curro, C. H. Wang, B. Hitti, G. Morris, E. D. Bauer, J. L. Sarrao, F. J. Litterst, and H.-H. Klauss, Phys. Rev. Lett. 103, 237003, (2009). 59. M. Mierzejewski, A. Ptok, and M. M. Maśka, Phys. Rev. B. 80, 174525, (2009). 60. Y. Yanase and M. Sigrist, J. Phys. Soc. Jpn. 78, 114715, (2009). 61. G. Koutroulakis, J. M. D. Stewart, V. F. Mitrović, M. Horvatić, C. Berthier, G. Lapertot, and J. Flouquet, Phys. Rev. Lett. 104, 087001, (2010). 62. R. Lortz, Y. Wang, A. Demuer, P. H. M. Böttger, B. Bergk, G. Zwicknagl, Y. Nakazawa, and J. Wosnitza, Phys. Rev. Lett. 99, 187002, (2007). 63. J. Singleton, J. Symington, M. Nam, A. Ardavan, M. Kurmoo, and P. Day, J. Phys.: Condens. Matter. 12, L641, (2000). 64. M. Tanatar, T. Ishiguro, H. Tanaka, and H. Kobayashi, Phys. Rev. B. 66, 134503, (2002). 65. S. Uji, H. Shinagawa, T. Terashima, T. Yakabe, Y. Terai, M. Tokumoto, A. Kobayashi, H. Tanaka, and H. Kobayashi, Nature. 410, 908, (2001). 66. L. Balicas, J. S. Brooks, K. Storr, S. Uji, M. Tokumoto, H. Tanaka, H. Kobayashi, A. Kobayash, V. Barzykin, and L. P. L. P. Gor’kov, Phys. Rev. Lett. 87, 067002, (2001). 67. V. Jaccarino and M. Peter, Phys. Rev. Lett. 9, 290, (1962). 68. S. Uji, T. Terashima, M. Nishimura, Y. Takahide, T. Konoike, K. Enomoto, H. Cui, H. Kobayashi, A. Kobayashi, H. Tanaka, M. Tokumoto, E. S. Choi, T. Tokumoto, D. Graf, and J. S. Brooks, Phys. Rev. Lett. 97, 157001, (2006). 69. L. Bulaevskii, A. Buzdin, and M. Maley, Phys. Rev. Lett. 90, 067003, (2003). 70. K. Cho, B. E. Smith, W. A. Coniglio, L. E. Winter, C. C. Agosta, and J. Schlueter, Phys. Rev. B. 79, 220507(R), (2009). 71. S. Yonezawa, S. Kusuba, Y. Maeno, P. Auban-Senzier, C. Pasquier, and D. Jérome, J. Phys. Soc. Jpn. 77, 054712, (2008). 72. J. Müller, M. Lang, R. Helfrich, F. Steglich, and T. Sakai, Phys. Rev. B. 65, 140509, (2002). 73. J. Wosnitza, S. Wanka, J. Hagel, M. Reibelt, D. Schweitzer, and J. Schlueter, Synth. Met. 133-134, 201, (2003). 74. H. Elsinger, J. Wosnitza, S. Wanka, J. Hagel, D. Schweitzer, and W. Strunz, Phys. June 30, 2010 4:39 30 World Scientific Review Volume - 9.75in x 6.5in Gertrud Zwicknagl and Jochen Wosnitza Rev. Lett. 84, 6098, (2000). 75. B. Bergk, A. Demuer, I. Sheikin, Y. Wang, J. Wosnitza, Y. Nakazawa, and R. Lortz, Physica C. in press, arXiv:0907.3769, (2010). 76. C. L. Chien and D. H. Reich, J. Magn. Magn. Mat. 200, 83, (1999). 77. E. A. Demler, G. Arnold, and M. R. Beasley, Phys. Rev. B. 55, 15174, (1997). 78. J. S. Jiang, D. Davidović, D. H. Reich, and C. L. Chien, Phys. Rev. Lett. 74, 314, (1995). 79. Z. Radović, M. Ledvij, L. Dobrosavljević-Grujić, A. I. Buzdin, and J. R. Clem, Phys. Rev. B. 44, 759, (1991). 80. I. A. Garifullin, D. A. Tikhonov, N. N. Garif’yanov, L. Lazar, Y. V. Goryunov, S. Y. Khlebnikov, L. R. Tagirov, K. Westerholt, and H. Zabel, Phys. Rev. B. 66(2), 020505 (2002). 81. V. Zdravkov, A. Sidorenko, G. Obermeier, S. Gsell, M. Schreck, C. Müller, S. Horn, R. Tidecks, and L. R. Tagirov, Phys. Rev. Lett. 97, 057004, (2006). 82. A. S. Sidorenko, V. I. Zdravkov, A. Prepelitsa, C. Helbig, Y. Luo, S. Gsell, M. Schreck, S. Klimm, S. Horn, L. R. Tagirov, and R. Tidecks, Ann. Phys. 12, 37, (2003). 83. L. R. Tagirov, Physica C. 307, 145, (1998). BCS50FFLO